wavelength dependent photochemical charge transfer at the osterloh/pubs/103.pdf¢ 2020....
Post on 20-Jan-2021
Embed Size (px)
This journal is©The Royal Society of Chemistry 2018 Chem. Commun., 2018, 54, 9023--9026 | 9023
Cite this:Chem. Commun., 2018, 54, 9023
Wavelength dependent photochemical charge transfer at the Cu2O–BiVO4 particle interface – evidence for tandem excitation†
Zongkai Wu, Ghunbong Cheung, Jiarui Wang, Zeqiong Zhao and Frank E. Osterloh *
The understanding of the photochemical charge transfer properties
of powdered semiconductors is of relevance to artificial photo-
synthesis and the production of solar fuels. Here we use surface
photovoltage spectroscopy to probe photoelectrochemical charge
transfer between bismuth vanadate (BiVO4) and cuprous oxide
(Cu2O) particles as a function of wavelength and film thickness.
Optimized conditions produce a �2.10 V photovoltage under 2.5 eV (0.1 mW cm�2) illumination, which suggests the possibility
of a water splitting system based on a BiVO4–Cu2O direct contact
The photoelectrochemical water splitting reaction can provide hydrogen fuel from only solar energy and water. To generate the required water electrolysis potential of approximately 1.6 V, two or more mid gap semiconductors are typically used in series.1,2
The ideal limiting solar to hydrogen efficiency of a dual absorber configuration (28%)3–5 is about twice that of a single absorber system.2–9 Tandem devices for the water splitting reaction often rely on monolithic absorber stacks10–19 that are difficult and expensive to fabricate because they require slow vacuum deposi- tion methods, such as metal organic chemical vapour deposition (MOCVD). This problem is avoided in particle based tandem systems, where the Ohmic contact between the light absorbers is established through soluble redox couples, I3
�/I�, or Fe3+/Fe2+, or through direct physical contact. Examples for this type of tandem system include suspended TiO2 particles,
20 tandems made of SrTiO3:Ru–BiVO4,
21,22 the ZrO2/TaON and WO3 tandem system,23,24 and the RuO2–TaON and Pt–TaON overall water splitting system.25–27 While particle contacts are easy to manu- facture, photochemical charge transfer dynamics at these ‘rough’ interfaces and their dependence on surface morphology, electro- lyte environment,28 and particle size are not well understood. As particles get smaller, the effect of internal electric fields
(space charge layers) diminishes, and charge transfer is domi- nated by the relative concentrations of the charge carriers, the energetics of the donor and acceptor configuration, and by surface and interfacial states of the particles.29 Understanding these factors is important for raising the energy conversion efficiency of particle-based systems. Here we use surface photo- voltage spectroscopy (SPS) to study photochemical charge transfer at the interfaces of Cu2O and BiVO4 nanoparticles. In SPS, the contact potential difference (CPD) of a sample film is measured under illumination with a semi-transparent Kelvin probe.30–33 A photovoltage (DCPD) can result from the movement of the charge carriers through the film or from their transfer across the interface between the particle film and a conductive substrate.34,35 This provides information about the majority carrier type, intermediate states, and the effective band gap of the semiconductor, with high sensitivity.29,34–36 We chose n-BiVO4 for this study because it is a known photoanode
and photocatalyst material for water oxidation under 2.5 eV bandgap illumination.23,43–45 As second absorber, p-Cu2O (2.1 eV) is used because it is a promising photocathode material for tandem PEC devices.46,47 As we show in the following, a tandem junction is formed at the BiVO4–Cu2O interface by simply layering these nanoparticles and by mildly annealing at 350 1C. This suggest the possibility of artificial photo- synthetic system based on powders of these two materials. It may also explain the improved photocatalytic dye degradation performance of Cu2O/BiVO4 composites previously reported in the literature.48–50 Cu2O nanoparticles for the study were synthe- sized from copper(II) acetylacetonate in acetone (details in ESI†).51 The reaction affords Cu2O nanoparticles in the Cuprite structure type with an average size of 59� 17 nm (XRD in Fig. S1, ESI†) and cubic microcrystals, with 1 mm edge length (Fig. 1B and C). Based on TEM images, the mass ratio of both particle sizes is 1 : 1. The BiVO4 nanoparticles for the study were synthesized from Bi2O3 and V2O5 in acetic acid, using a revised method.49 The material crystallizes in the Scheelite structure type (Fig. S1, ESI†) and forms particles of 73 � 35 nm average size (Fig. 1A and D).
Department of Chemistry, University of California, Davis. One Shields Avenue,
Davis, CA, 95616, USA. E-mail: firstname.lastname@example.org; Fax: +1 530 752 8995 † Electronic supplementary information (ESI) available: Experimental details, XRD, SEM and UV/vis data. See DOI: 10.1039/c8cc04123g
Received 24th May 2018, Accepted 19th July 2018
http://orcid.org/0000-0001-6988-4324 http://orcid.org/0000-0002-9288-3407 http://crossmark.crossref.org/dialog/?doi=10.1039/c8cc04123g&domain=pdf&date_stamp=2018-07-26 http://rsc.li/chemcomm
9024 | Chem. Commun., 2018, 54, 9023--9026 This journal is©The Royal Society of Chemistry 2018
Thin films of the particles were prepared by drop-casting suspensions on FTO substrates, followed by drying in air and annealing at 350 1C under argon for 5 h. These films have a red- brown (Cu2O) or yellow (BiVO4) appearance and contain the particles in loosely packed form (Fig. 1C and D and insets). Surface photovoltage and optical spectra for separate BiVO4 and Cu2O particle films on FTO are presented in Fig. 2. The spectrum for BiVO4 contains a negative photovoltage feature that can be attributed to photoinduced electron transport to the FTO substrate, as expected for an n-type semiconductor.52 The 2.45 eV onset is slightly below the 2.55 eV optical absorption onset of the material (Fig. 2), which is attributed to tail states near the band edges. In contrast, the photovoltage signal for the Cu2O particle film on FTO has a positive sign. Here, the voltage results from injection of hole majority carriers into the FTO substrate. The onset energy of 2.0 eV corresponds well with the major absorption feature of the material and to the optical band gap reported in the literature.56
The photovoltage spectra can be understood on the basis of the energetics of the FTO/sample configurations, as shown in Fig. 3A and B. Fundamentally, the photovoltage of a particle film is determined by the offset of the FTO workfunction (Fermi energy) and the band edges of the light absorber. These offsets are +0.3 V and �0.35 V for Cu2O and BiVO4 on FTO, respectively. The experimentally observed photovoltage values (+70 mV for Cu2O and�165 mV for BiVO4) are lower, which is attributed mainly to the low light intensity of the light source (0.1 to 0.3 mW cm�2). For example, in a previous study the photovoltage was found to vary
with the logarithm of the light intensity.34,53 Another reason is that the sample film thickness is below the optical absorption depth of each material (see discussion below).
Next, to evaluate photochemical charge transfer between Cu2O and BiVO4, a stacked particle film was assembled by two sequential drop-casting steps each followed by annealing in argon at 350 1C. Scanning electron micrographs of the stacked film are shown in Fig. 1E and EDS analysis results are shown in Fig. 1F and Fig. S2 (ESI†). Two distinct 3–5 micrometer thick layers of BiVO4 nanoparticles at the top and loosely packed Cu2O nano- and microparticles at the bottom can be observed. Elemental mapping confirms the composition of each layer with no particle intermixing occurring. Surface photovoltage
Fig. 1 Transmission electron microscope images for (A) BiVO4 and (B) for Cu2O particles. Scanning electron microscope images for (C) Cu2O single layer, top view (photo in insert) and (D) BiVO4 single layer, top view (photo in inset). (E) FTO–BiVO4–Cu2O double layer, cross view. (F) Energy-dispersive X-ray spectroscopy (EDS) element map overlaid onto SEM image.
Fig. 2 Surface photovoltage spectra and diffuse reflectance optical absorption spectra of (A) 0.80 micrometer thick BiVO4 film on fluorine doped tin oxide (FTO), and (B) 0.72 micrometer thick Cu2O film on FTO. KM stands for Kubelka–Munk.
Fig. 3 Energy scheme for (A) FTO/Cu2O and FTO/BiVO4 single layer films and (B) energy scheme for FTO/Cu2O/BiVO4 bilayer film using band edges from the literature.44,46
This journal is©The Royal Society of Chemistry 2018 Chem. Commun., 2018, 54, 9023--9026 | 9025
spectra for FTO/Cu2O/BiVO4 stacks are shown in Fig. 4. Layer thicknesses were chosen in the 1.25 to 5 mm range to ensure optimal light absorption and charge transport. In all cases, a strongly negative photovoltage is observed above 2.25 eV. This voltage reaches a maximum around 2.5 eV where both materials can absorb light strongly (Fig. 4A), and then decays at higher photon energies, due to the decrease in light penetration depth at higher photon energy. The sign of the voltage and its size indicates that both absorbers now act in tandem, as shown in the excitation scheme in Fig. 3B. Holes from Cu2O are no longer injected into the bottom FTO but into the top BiVO4 layer where they recombine with majority carriers formed under BiVO4 excitation. This reversal of the charge transfer direction in the Cu2O particle layer is attributed to the